A l l - C e r a m i c Sy s t e m s :Laboratory andClinical PerformancePetra C. Guess, DDS, Dr Med Denta,*, Stefan Schultheis, DDS, Dr Med Denta,Estevam A. Bonfante, DDS, MSc, PhDb, Paulo G. Coelho, DDS, PhDc,Jonathan L. Ferencz, DDSd, Nelson R.F.A. Silva, DDS, MSc, PhDd KEYWORDS All-ceramic material CAM/CAD Zirconia AluminaOver the last 3 decades, a trend to shift toward metal-free restorations has beenobserved in the dental field. To meet the increased demands of patients and dentistsfor highly aesthetic, biocompatible, and long-lasting restorations, several types of all-ceramic systems have been developed.1 Silicate and glass ceramics are used asa veneer for metal or all-ceramic cores to optimize form and aesthetics. In a monolithicapplication, small-sized restorations such as inlays, onlays, laminate veneers, andcrowns can also be fabricated. High-strength ceramics such as aluminum and zirco-nium oxide ceramics were developed as a core material for crowns and fixed dentalprostheses (FDPs) to extend the indication ranges to the high-load bearing areas.2Most recently, monolithic zirconia restorations are increasingly promoted for single-crown and full-mouth rehabilitation, in particular for patients with parafunctionalhabits. Because of advances in computer aided design (CAD) and computer aidedmanufacturing (CAM) technologies, the high-strength ceramic systems have becomeincreasingly popular. Zirconia, specifically yttria-containing tetragonal zirconia poly-crystal (Y-TZP), with unsurpassed mechanical properties (Table 1), has had its clinicalapplication expanded from single crowns and short-span FDPs to multiunit and full-arch zirconia frameworks as well as to implant abutments and complex implant super-structures to support fixed and removable prostheses.3,4 Zirconia in its pristine formcan be considered as a reliable framework material with reported failure rates lower a Department of Prosthodontics, Dental School, Albert-Ludwigs University, Hugstetter Street 55, 79106 Freiburg, Germany b Department of Prosthodontics, UNIGRANRIO University, School of Dentistry, Rio de Janeiro, Brazil c Department of Biomaterials and Biomimetics, New York University College of Dentistry, New York, NY, USA d Department of Prosthodontics, New York University College of Dentistry, New York, NY, USA * Corresponding author. E-mail address: email@example.com Dent Clin N Am 55 (2011) 333–352 doi:10.1016/j.cden.2011.01.005 dental.theclinics.com 0011-8532/11/$ – see front matter Ó 2011 Elsevier Inc. All rights reserved.
334 Guess et al Table 1 Mechanical properties of different all-ceramic systems according to manufacturer’s instructions Modulus Hardness Toughness Strength CTE C Material (GPa) (GPa) (MPa m1/2) (MPa) X 3 10L6 Firing ( C) Porcelain Vitablocks 45 NA NA 154 9.4 780–790 (feldspathic) Lava Ceram 78 5.3 1.1 100 10.5 810 IPS e.max ceram 60–70 5.4 NA 90 9.5 750 IPS e.max ZirPress 65 5.4 NA 110 10.5–11 900–910 (flour-apatite) Glass-ceramic Dicor 75 3.4 1.4 290 9.8 850 Empress esthetic 65–68 6.2 1.3 160 16.6–17.5 625 (leucite) IPS e.max Press 95 5.8 2.75 400 10.2–10.5 915–920 (lithium disilicate) IPS e.max CAD 95 5.8 2.25 360 10.2–10.5 840 (lithium disilicate) Alumina In-Ceram Alumina 280 20 3.5 500 7.2 2053 melting point Procera Alumina 340 17 3.2 695 7.0 1600 Zirconia Cercon 210 12 9 1300 10.5 1350 IPS e.max 210 13 5.5 900 10.8 1500 Zir CAD Lava 210 14 5.9 1048 10.5 1480 DSC Zirkon 210 12 7 1200 10.4 1500 In-Ceram YZ 210 12 5.9 900 10.5 2706 melting point Procera Zirconia 210 14 6 1200 10.4 1550 Prettau Zirkon 210 12.5 NA 1000 10 1600 Zirkonzahn Tooth Dentin 16 0.6 3.1 — 11–14 — Enamel 94 3.2 0.3 — 2–8 — Abbreviations: CTE, coefficient of thermal expansion; NA, not available. than those observed for silicate or alumina frameworks (Table 2).5 However, questions regarding the overall success of bilayer zirconia/veneer restorations have been raised as a result of early chipping/fracture events observed6 while in oral function. As a result, various research groups have tried to better understand the potential prob- lems such as the thermal interaction between the ceramic core and veneering porce- lain, their respective processing techniques, and the effect of framework configuration on veneer support, in an attempt to overcome early chippings/fractures and enhance the long-term service of all-ceramic systems.
All-Ceramic Systems 335 This overview presents the current knowledge of monolithic and bilayer all-ceramicsystems and addresses composition and processing mechanisms, laboratory andclinical performance, and possible future trends.REINFORCED GLASS CERAMICSThe interest in nonmetallic and biocompatible restorative materials increased after theintroduction of the feldspathic porcelain crown in 1903 by Land.7 In 1965, McLean8pioneered the concept of adding aluminum oxide to feldspathic porcelain in anattempt to enhance mechanical properties. However, the clinical shortcomings ofthese materials, such as brittleness, crack propagation, low tensile strength, wearresistance, and marginal accuracy, discontinued its use.9 Increased strength in glassy ceramics can be achieved by adding appropriate fillersthat are uniformly dispersed throughout the glass, a technique termed dispersionstrengthening. Leucite is used as a reinforcing crystalline at a concentration of 35 to45 vol%.10 In the early 1990s, the lost wax press technique was introduced to dentistryas an innovative processing method for all-ceramic restorations. Examples of leucite-reinforced glass ceramics are VITA VMK 68 (VITA Zahnfabrik, Bad Sackingen, ¨Germany), Finesse All-Ceramic, (Dentsply, York, PA, USA), Optec OPC (Jeneric, Wall-ingford, CT, USA), and IPS Empress (Ivoclar Vivadent, Schaan, Principality ofLiechtenstein). The molding procedure of IPS Empress is conducted at 1080 C ina special, automatically controlled furnace. Leucite crystals are formed througha controlled surface crystallization process in the SiO2-Al2O3-K2O glass system.Tangential compressive stresses develop around the crystals on cooling because ofthe difference in the coefficient of thermal expansion (CTE) between leucite crystalsand the glassy matrix. These stresses contribute to crack deflection and improvedmechanical performance.11 IPS Empress, for instance, exhibits a flexural strength of120 to 180 MPa and a CTE of 15 to 18.5 Â 10À6 KÀ1 m/m.12 The material is suitablefor fabrication of inlays, onlays, veneers, and crowns. Favorable clinical long-termdata with high survival rates are described for IPS Empress inlays, onlays (90% after8 years13), veneers (94.4% after 12 years14), and crowns (95.2% after 11 years15) in thedental literature. Leucite glass ceramics can also be machined with various CAD/CAM systems. Multi-colored blocks were recently developed to reproduce color transitions and shading aswell as different levels of translucency to reproduce natural teeth (Fig. 1).16 The use ofleucite-reinforced glass ceramic has significantly declined because of the introductionof lithium disilicate glass ceramics with significantly improved mechanical andaesthetic properties and is addressed in detail in the next section.LITHIUM DISILICATE GLASS CERAMICSA significantly higher strength of 350 MPa was achieved with a glass ceramic of theSiO2-Li2O-K2O-ZnO-P2O5-Al2O3-La2O3 system by precipitating lithium disilicate(Li2Si2O5) crystals. The crystal content of up to 70 vol% is considerably higher thanthat of leucite materials.11 High-temperature x-ray diffraction studies revealed thatboth lithium metasilicate (Li2SiO3) and crystobalite form during the crystallizationprocess before the growth of lithium disilicate (Li2Si2O5) crystals.17 The final micro-structure consists of highly interlocked lithium disilicate crystals, 5 mm in length and0.8 mm in diameter. Thermal expansion mismatch between lithium disilicate crystalsand glassy matrix results in tangential compressive stresses around the crystals,potentially responsible for crack deflection and strength increase. Crystal alignmentafter heat pressing of the lithium disilicate glass ceramic leads to multiple crack
336 Guess et alTable 2Clinical outcomes of zirconia-based crowns and FDPs Observation Sample Survival Framework VeneerStudy Ceramic Materials Period (y) Type of Restoration Size Rate (%) Fracture (%) Fracture (%)Cehreli et al,61 2009 Cercon 2 Single crowns 15 NS 7 0 Veneer n.s.Groten Huttig,108 2010 Cercon 2 Single crowns 54 98 0 9 Cercon Ceram KissOrtorp et al,68 2009 Noble Procera Zirconia 3 Single crowns 204 92.7 0 2 Vita Lumin Noble Rondo ZirconiaSchmitt et al,109 2010 Lava 3 Single crowns 19 100 0 5 Lava CeramSchmitter et al,67 2009 Cercon 2 4- to 7-unit FDP 30 96.6 3 3 Cercon Ceram STsumita et al,110 2010 Cercon 2 3-unit FDP 21 NS 0 14 Creation ZISailer et al,69 2009 Cercon 3 3- to 5-unit FDP 38 100 0 25 Cercon Ceram SBeuer et al,63 2009 Cercon 3 3-unit FDP 21 90.5 5 0 Cercon Ceram ExpressRoediger et al,64 2010 Cercon 4 3- to 4-unit FDP 99 94 1 13 Cercon Ceram S Experimental veneering ceramicWolfart et al,75 2009 Cercon 4 3- to 4-unit 24 96 0 13 Cercon Ceram S FDP/Cantilever FDP 34 92 0 12 Cercon Ceram Express
Sailer et al,62 2007 Cercon 5 3- to 5-unit FDP 57 73.9 8 15 Experimental veneering ceramic Crisp et al,111 2008 Lava 1 3- to 4-unit FDP 38 100 0 3 Lava Ceram Raigrodski et al,112 2006 Lava 2.5 3-unit FDP 20 NS 0 25 Veneer n.s. Schmitt et al,113 2009 Lava 3 3- to 4-unit FDP 27 100 0 11 Lava Ceram Vult von Steyern et al,114 2005 DC Zirkon 2 3- to 5-unit FDP 20 NS 0 15 Vita D Tinschert et al,83 2008 DC Zirkon 3 3- to 10-unit 65 NS 0 6 Vita D FDP/Cantilever FDP Edelhoff et al,115 2008 Digident 3 3- to 6-unit FDP 21 90.5 0 10 Initial ZirKeramik GC Molin and Karlsson,116 2008 Denzir 5 3-unit FDP 19 100 0 36 Vita D IPS Empress Nothdurft Pospiech,84 2009 Cercon 0.5 Implant-supported 40 NS 0 8 Cercon Ceram Kiss single crowns Larsson et al,49 2006 Denzir 1 Implant-supported 13 NS 0 53 Esprident Triceram FDP Larsson et al,3 2010 Cercon 3 Implant-supported 10 100 0 34 Cercon Ceram S full-arch FDP All-Ceramic SystemsAbbreviation: NS, not specified. 337
338 Guess et al Fig. 1. Before and after treatment with all-ceramic restorations (lithium disilicate IPS e.max Press Tooth 24 inlay; onlays 26, 27; and crowns14, 15, 25) and CAD/CAM-fabricated leucite ProCAD onlay 16, 26. deflections. The lithium disilicate ceramic was introduced as IPS Empress 2 (Ivoclar Vivadent) in 1998 and is moldable as leucite glass ceramics, but at a lower tempera- ture of 920 C. The CTE is 10.5 Â 10À6 KÀ1 m/m.18 High survival rates were observed for anterior and posterior IPS Empress 2 crowns (95.5% after 10 years19) in long-term clinical studies (Fig. 2). The clinical success of 3- unit IPS Empress 2 FDPs is predominately limited by bulk fracture failure within the connector area, in particular when the connector size is less than the recommended dimensions (70% survival rate after 5 years20) (Fig. 3). A newly developed pressable lithium disilicate glass ceramic (IPS e.max Press, Ivo- clar Vivadent) with improved physical properties (flexural strength, 440 MPa) and translucency through different firing process has been developed in the SiO2-Li2O- K2O-ZnO-P2O5-Al2O3-ZrO2 system. The pressable lithium disilicate ceramic can be used in monolithic application for inlays, onlays, and posterior crowns or as a core material for crowns and 3-unit FDPs in the anterior region. Apatite glass ceramics are recommended for veneering. Fig. 2. Lithium disilicate crowns (IPS Empress 2) at baseline and functionally and aestheti- cally successful performance after 5 years.
All-Ceramic Systems 339Fig. 3. Three-unit lithium disilicate (IPS Empress 2) FDPs at baseline and a connector bulkfracture after 11 months. Clinical data exhibited high survival rates on IPS e.max Press onlays (100% after3 years),21 crowns (96,6% after 3 years),22 monolithic inlay retained FDPs (100% after4 years),23 and full crown retained FDPs (93% after 8 years).24 Recently, a lithium disilicate glass ceramic (IPS e.max CAD, Ivoclar Vivadent) hasbeen designed for CAD/CAM processing technology. The milled lithium disilicate blockis exposed to a 2-stage crystallization process. Lithium metasilicate crystals areprecipitated during the first stage. The resulting glass ceramic has a crystal size rangeof 0.2 to 1.0 mm with approximately 40 vol% lithium metasilicate crystals. At this pre-crystallized state, the CAD/CAM block exhibits a flexural strength of 130 to 150 MPa,which allows simplified machining and intraoral occlusal adjustment. The final crystal-lization process occurs after milling of the restoration at 850 C in vacuum. The meta-silicate crystal phase is dissolved completely, and the lithium disilicate crystallizes.This process also converts the blue shade of the precrystallized block to the selectedtooth shade and results in a glass ceramic with a fine grain size of approximately 1.5 mmand a 70% crystal volume incorporated in a glass matrix.16 CAD/CAM-processedlithium disilicate glass ceramic demonstrates a flexural strength of 360 MPa (seeTable 1). Because of the favorable translucency and shade assortment the materialcan be used for fully anatomic (monolithic) restorations with subsequent staining char-acterization or as a core material with subsequent coating with veneering ceramics.The manufacturer recommends its use for anterior or posterior crowns, implantcrowns, inlays, onlays, and veneers. Preliminary clinical results on single crownsrevealed high survival rates (100% after 2 years25) and are hence extremely promising.GLASS-INFILTRATED CERAMICSAnother group of all-ceramic systems involves glass-infiltrated ceramics. In-CeramAlumina (VITA Zahnfabrik) was the first all-ceramic system available for single-unitrestorations and 3-unit anterior bridges26 with a high-strength ceramic core fabricatedwith the slip-casting technique.27 A slurry of densely packed (70–80 wt%) Al2O3 isapplied and sintered to a refractory die at 1120 C for 10 hours.28,29 This processproduces a porous skeleton of alumina particles, which is infiltrated with lanthanum
340 Guess et al glass in a second firing at 1100 C for 4 hours to eliminate porosity and increase strength.29 The core is veneered with feldspathic porcelain.26 In-Ceram Zirconia (VITA Zahnfabrik) is a modification of the original In-Ceram Alumina system, with an addition of 35% partially stabilized zirconia oxide to the slip composition to strengthen the ceramic.27 Traditional slip-casting techniques can be used, or the material can be copy-milled from prefabricated, partially sintered blanks and then veneered with feld- spathic porcelain.30 As the core is opaque and lacks translucency, the use of this mate- rial for anterior regions becomes problematic.27 Clinical performance of glass-infiltrated ceramics for crowns and FDPs indication has been evaluated in a systematic review.31 However, with the development of high-strength ceramics, recent literature on glass- infiltrated ceramics became sparse. HIGH-STRENGTH OXIDE CERAMICS Although high-strength ceramic in dentistry includes alumina and zirconia, this section focuses mainly on zirconia because of its superior mechanical properties compared with alumina and the current controversial aspects of its clinical performance. Zirconia ceramics have gained a remarkable interest in biomedical sciences.4 The first reference concerning their application in medicine appeared in the late sixties; 20 years later, Christel and colleagues32 studied their use in orthopedic surgery.33 In the early 1990s, zirconia was introduced to dentistry,34 and in recent years, a large number of publications appeared in the literature. Zirconia, characterized by a dense, monocrystalline homogeneity, possesses low thermal conductivity, low corrosion potential, and good radiopacity.4 High biocompat- ibility, low bacterial surface adhesion, and favorable optical properties of zirconia ceramics are reported.35–37 Zirconia in its pure form is a polymorph that has 3 temperature-dependant phases that are monoclinic (room temperature to 1170 C), tetragonal (1170 C–2370 C), and cubic (2370 C to melting point).34 With the addition of stabilizing oxides such as magnesia, ceria, yttria, and calcium to zirconia, the tetrag- onal phase is retained in a metastable condition at room temperature, enabling a phenomenon called transformation toughening to occur. In response to mechanical stimuli, the partially stabilized crystalline tetragonal zirconia transforms to the more- stable monoclinic phase, with a local volume increase of approximately 4%. This increase in volume counteracts further crack propagation by compression at the tip of the crack.38 Compared with high-strength alumina ceramic, zirconia has twice the flexural strength (900–1200 MPa).39,40 In addition, high fracture toughness (9–10 MPa∙m1/2) has been described.39 The most commonly used dental zirconia formulations are glass-infiltrated zirconia toughened alumina ceramics (In-Ceram, VITA Zahnfabrik) and 3 mol% Y-TZP. Y-TZP has been used for root canal posts,41 frameworks for posterior teeth, implant-supported crowns, multiunit FDPs,42 resin- bonded FDPs,43 custom-made bars to support fixed and removable dental prostheses,44 implant abutments,45,46 and dental implants.47,48 A magnesium-doped partially stabilized zirconia (Mg-PSZ, Denzir M, Dentronic AB, Sweden) is available, but porosity and large grain size has limited its success.49 Zirconia and CAD/CAM Technology An array of CAD/CAM systems has evolved since F. Duret introduced the concept in 1971.50,51 Some CAD/CAM systems (Denzir, Cadesthetics, Skelleftea, Sweden, and ˚ DC-Zircon, DCS Dental AG, Allschwil, Switzerland) machine fully sintered Y-TZP blocks, which have been processed by hot isostatic pressing. Because of the hard- ness and poor machinability of fully sintered Y-TZP, a robust milling system and
All-Ceramic Systems 341extended milling periods are required. Most of the available CAD/CAM systems shapeblocks of partially sintered zirconia.34 Milling from partially sintered blocks involvesmachining enlarged frameworks in a so-called green state. These blocks are thensintered to their full strength, which is accompanied by shrinkage of the milled frame-work by approximately 25% to the desired dimensions. Examples of these systemsare CERCON (Dentsply Friadent, Mannheim, Germany), LAVA (3M ESPE, Seefeld,Germany), Procera (Nobel Biocare, Gothenburg, Sweden), Etkon (Straumann, Basel,Switzerland), and Cerec (Sirona, Bensheim, Germany). The advantage of industrialized blank fabrication and reproducible and consistentCAM resulted in increased process reliability and cost-effectiveness of CAD/CAM-fabricated restorations.52 Labor-intensive waxing, casting, and soldering of frame-works accompanied with conventional laboratory procedures can be avoided withthe application of CAD/CAM technology. With extensive frameworks, particularlyused in implant dentistry, and the escalating costs of precious alloys, all-ceramicrestorations are competitive with conventional metal-ceramic restorations (MCRs)from a cost perspective.53Zirconia and Low-Temperature DegradationA major drawback of zirconia restorations compared with metal-ceramics is thematerial-inherent accelerated aging that has been observed to occur in zirconia inthe presence of moisture.54,55 This aging phenomenon is known as low-temperaturedegradation (LTD) and was first described by Kobayashi and colleagues56 in 1981.At relatively low temperatures (150 C–400 C), slow tetragonal to monoclinic transfor-mations occur, initiating at the surface of polycrystalline zirconia and subsequentlyprogressing into the bulk of the material.34,57 Transformation of 1 grain is accompa-nied by an increase in volume, which causes stress on the surrounding grains andmicrocracking. Water penetration into these cracks then exacerbates the process ofsurface degradation, and the transformation progresses. The growth of the transfor-mation zone results in severe microcracking, grain pullout, and finally surface rough-ening, which ultimately leads to strength degradation. Any factor that is detrimental tothe stability of tetragonal zirconia is susceptible to promote LTD. Among these factorsare grain size,58 the amount of stabilizer,59 and the presence of residual stress.54,60 Atpresent, there is no clear correlation between LTD and failure predictability whenzirconia is used as a dental bioceramic.33Clinical Data on Zirconia-Supported RestorationsAlthough zirconia was introduced to dentistry in the early 1990s, limited information aboutits clinical performance can be found. A literature search from 1990 through September2010 using electronic databases (PubMed and MEDLINE) revealed a total of 21 clinicaltrials on zirconia-supported restorations (see Table 2). Long-term clinical data forzirconia-supported restorations with observation periods exceeding 5-year time framesare not yet available. Most studies (n 5 14) investigated predominately posterior FDPs,whereas a small number focused on (n 5 4) crowns. Only 3 studies described the clinicalbehavior of implant-supported zirconia-supported FDPs and single crowns.Veneered Zirconia Clinical Failure ModesCore/framework fracturesCatastrophic fractures within the zirconia core ceramic are reported at 7% forsingle crowns after 2 years and at 1% to 8% for FDPs after 2 to 5 years (seeTable 2). Occlusal overloading caused by bruxism (crown fracture after 1 month61)or trauma (connector fracture 5-unit FDP after 38 months62) and insufficient framework
342 Guess et al thickness at 0.3 mm (crown-abutment fractures in 3-unit FDP63,64) were mentioned as the main reasons for zirconia core bulk fractures. Fractographic analyses of clinically failed zirconia crowns showed that radial fractures propagating upwards from the cementation surface site resulted in bulk fractures and caused catastrophic failures of the restorations.65 Microscopic examinations of failed zirconia-based FDPs revealed that core bulk fractures were most commonly located in the connector area and initiated from the gingival surface, where tensile stresses were the greatest because of occlusal loading.65,66 Core bulk fracture in the connector area was also attributed to damage induced during fabrication.67 A higher susceptibility to connector fracture was noted with an increased span of FDPs.65 Veneering ceramic cohesive fractures The major drawbacks noted in all clinical studies on zirconia-supported restorations were less related to the framework integrity than to wear and failure of the veneering ceramics. Cohesive fractures within the veneering ceramic (chipping) were described as the most frequent reason for failures, irrespective of the applied zirconia veneer system (see Table 2). Veneer fracture rates are reported at 2% to 9% for single crowns after 2 to 3 years and at 3% to 36% for FDPs after 1 to 5 years. Implant-supported zirconia-based restorations revealed even higher rates at 8% for single crowns after 6 months and at 53% for FDPs after 1 year. Impaired proprioception and rigidity of osseointegrated implants correlated with higher functional impact forces might further exacerbate cohesive veneer fractures. To date, only one 3-year prospective clinical study involving implant-supported full-arch Y-TZP reconstructions is available. Despite the short follow-up period and limited number of patients (n 5 10), no frame- work fractures were observed; however, chip-off fractures were observed in 34% of the units cemented in 9 of 10 patients.3 Depending on the size and localization, cracks leading to veneer fractures can severely compromise the aesthetics and function of zirconia-supported restorations.68,69 Fracto- graphic analysis of clinically failed veneered zirconia restorations revealed cohesive veneer failures, with cracks originating from the occlusal surface and propagating to the core veneer interface, leaving an intact core.65 In many clinical studies, it seemed that these veneer failures were associated with roughness in the veneering ceramic because of occlusal function or occlusal adjustment.49,69,70 Therefore, special attention has to be paid to the static and dynamic aspects of occlusion in zirconia-based restora- tions. Occlusal adjustments should be performed only with fine-grain diamonds under water irrigation followed by a thorough polishing sequence. Reasons for veneering ceramic failure As the veneering ceramic material (flexural strength, approximately 90–120 MPa) is weak compared with the high-strength core material (900–1200 MPa),39,40 the veneering ceramic seems to be prone to failure at low loads during masticatory func- tion. The use of higher-strength veneering ceramic was proposed to reduce the incidence of veneer chippings/fractures. However, attempts to improve the micro- structure and mechanical properties of veneering ceramics with the development of glass-ceramic ingots for pressing veneering ceramics onto zirconia frameworks did not result in an increased reliability of the veneering ceramic.71,72 In addition, identical chip-failure patterns were observed.71–74 Although a high density of the veneering layer has been expected with the press technique, spherical porosities were noted within the veneer layer and also at the interface.72 In clinical trials on zirconia FDPs, chipping fractures have also been reported with pressable veneering ceramics, and the chipping problem does not seem to be solved.75
All-Ceramic Systems 343 Moreover, the CTE is frequently discussed as a contributing factor for veneer failure.However, the problem of chipping may not be limited only to the mismatch of CTE; itseems more complex. Residual stresses in bilayer crowns and FDPs are associatedwith the possibility of thermal gradients being developed in these structures duringcooling. For zirconia veneer all-ceramic systems, the low thermal conductivity of thezirconia (approximately 3 Wm/K)76 results in the highest temperature difference and,therefore, very high residual stresses. In addition, thick layers of veneering ceramicson zirconia cores are highly susceptible to generating high tensile subsurface residualstresses, ultimately resulting in unstable cracking or chipping.77 Slow cooling of therestoration above the glass transition temperature of the porcelain could preventthe development of high tensile subsurface residual stresses in the porcelain, whichmay result in unstable cracking or chipping. Most manufacturers now recommendthe approach of a reduced cooling rate after final firing or glazing, and even an addi-tional 6 minutes has shown to be effective.78Zirconia framework designThe lack of a uniform support of the veneering ceramic because of improper frame-work design has been discussed as a possible reason for chipping fractures. Remark-ably little scientific clinical data on optimal design of zirconia-supported restorationshave been published.53,79,80 With the introduction of CAD/CAM technologies indentistry, excessive veneer layer thickness (2.5 mm) was created because of theuniform layer thickness of the copings for crowns and bar-shaped connectorsfor FDPs. Improved customized zirconia coping design derived from the conventionalporcelain fused to metal technique has been recommended to provide adequatesupport for the veneering ceramic.80 A dual-scan procedure of the die and full-contour wax pattern has been merged to fabricate the desired framework. Preliminaryin vitro studies showed that cohesive fractures within the veneering ceramic could notbe avoided with the improved support, but the size of the fractures was significantlydecreased81,82 and failure initiation was shifted toward higher loads.73 In clinicalobservation, conflicting results on the framework design modification have beendescribed.83,84 Hence, the effect of framework design modifications on residual stressstates needs to be better elucidated.77Minimizing Zirconia Core FailuresSome fundamental aspects affecting the clinical performance of zirconia as a frame-work material need to be addressed. Laboratory technicians and clinicians shouldfollow the precise sequence steps in manufacturing zirconia-based restorations,with the knowledge that zirconia as a framework material is potentially damaged bysurface modifications and improper laboratory and clinical handling techniques.85 Grinding or sandblasting of surfaces with high (or mild/low) pressure ranges isimplicated as a factor in inducing the formation of surface microcracking85–87 thatcould be detrimental to the long-term performance of the restorations and lead tounexpected failures.88 Several research groups have claimed an increased flexuralstrength in Y-TZP89 because of phase transformation after grinding and aluminaabrasion.90–92 However, any temporary beneficial effect related to phase transforma-tion induced by different surface treatment methods may be negated by fatigue-related crack growth phenomena and following heat treatments associated withveneer application.90 With respect to the highly deleterious effect on zirconiareliability,93 postsintering surface modifications of zirconia frameworks at the dentallaboratory or under clinical circumstances should be avoided.
344 Guess et al LABORATORY PERFORMANCE OF ALL-CERAMIC MATERIALS Randomized prospective clinical trials are the first choice for evaluating clinical long- term behavior of dental materials and techniques. However, the results of clinical investigations are restricted by high costs, and meaningful conclusions can be drawn only if an adequate number of restorations are incorporated and observed for at least 3 to 4 years.94 In addition, fractures are occasionally observed after 4 to 5 years of clin- ical service (Ferencz J, personal communication, 2010). Therefore, in vitro simulations and laboratory tests are developed to investigate new dental materials and predict life- times and failures. Various testing methods have been used to investigate the mechanical properties of dental materials. Many concerns have been raised lately regarding the clinical signif- icance of simple traditional mechanical testing methodologies and single load to failure tests of dental restorations, loosely termed “crunch the crown test”95 or flexural strength tests. These tests report unrealistically high fracture strength values, largely overestimating the actual failure load. Furthermore, the obtained failure modes differ significantly from those reported in clinical observations. Hence, little insight into damage initiation and propagation can be provided.96 In material science, fatigue is the progressive and localized structural damage that occurs when a material is sub- jected to cyclic loading. Fatigue is a significant factor limiting the lifespan of zirconia-based restorations and, therefore, represents a prerequisite for valid in vitro testing.97 A recently developed mouth-motion fatigue model has demonstrated the ability to duplicate clinical fractures98 and predict the material’s reliability to validate its clinical potential. Guess and colleagues99 examined the failure and fatigue behavior of a hand-layer veneered zirconia core ceramic and compared it with a monolithic CAD/CAM- fabricated lithium disilicate ceramic. A sliding contact mouth-motion fatigue testing in water on anatomically correct crowns was applied to simulate approximating tooth surfaces during mastication. Hand-layer veneered zirconia crowns supported by tooth replicas revealed a high single-cycle load to failure strength of 1195 Æ 221 N. But during mouth-motion fatigue testing, hand-layer veneered zirconia-based crowns resulted in a very limited reliability; approximately 90% of specimens failed from veneer chip-off fracture by 100,000 cycles at 200 N. Failure progressed from the contact area through the body of the veneering ceramic as noted in clinical cases.65 The observed fatigue behavior of zirconia-supported crowns does not seem to be material or system dependent, as similar results were reported in previous findings using the identical test methodology.100 In contrast, CAD/CAM lithium disilicate crowns showed no failures up to load levels exceeding posterior physiologic chewing forces and seemed to be resistant to mouth-motion step-stress (900 N/180,000 cycles) and also to staircase fatigue (1000 N/1 million cycles).101 A threshold for damage and bulk fracture could be detected in the range of 1100 to 1200 N. CAD/CAM processing of the lithium disilicate ceramic uses industrialized fabricated homogenous ceramic blanks; there- fore, the material reveals a high density with a minimum of inherent flaws. Increased Weibull modulus and reliability have been reported for CAD/CAM-fabricated materials.102 Conversely, the presence of structural “impurities” within the veneer layer of zirconia-supported ceramics is a known drawback of bilayer all-ceramic systems.71 The Gold-Standard Metal-Ceramic Although MCRs are frequently referred to as the gold standard and still represent a common procedure to rehabilitate missing dental structures and teeth, limited infor- mation is available regarding their clinical and laboratory performance when
All-Ceramic Systems 345compared with all-ceramic systems. After the introduction of zirconia to dentistry,more elaborate clinical and laboratory investigations were performed, but MCRswere, in most instances, not included as control.103,104 Moreover, the understandingof the failure mechanisms of MCRs is mainly related to biological issues rather thanfracture or chipping of the veneer porcelain.105 In one of the few laboratory studies presented in the dental literature, Silva andcolleagues74 performed a sliding contact fatigue test study on anatomically correctMCR crowns and compared the reliability and failure modes with zirconia-supported crowns. Fig. 4 shows a series of representative images of laboratory-tested MCRs, zirconia-supported crowns, and its clinical-matched fractures. Theresemblance of failure modes for both systems shows the potential of use slidingFig. 4. Comparison between clinical and laboratory fractures. (A) Metal-ceramic molarcrown fractured after about 13 years of oral function. (B) Representative metal-ceramicmolar crown after step-stress mouth-motion fatigue test. White arrows in (A) and (B)show typical veneer cohesive fractures. (C) Typical clinical veneer cohesive fracture (blackarrow) at the proximal aspect of a Y-TZP-supported all-ceramic crown after 2.5 years inoral function. (D) Typical fracture (black arrow) at the proximal aspect of a Y-TZP-supportedall-ceramic crown after a mouth-motion fatigue test. Note similar fracture patterncompared with clinical failure mode shown in (C). ([A] Courtesy of Dr Carlo Marinello,University of Basel, Switzerland.)
346 Guess et al contact fatigue concept to preclinical scenarios. The investigators74 observed that the MCR system presented a significantly higher reliability compared with Y-TZP, which may explain the fact that not many reports of veneer fractures for MCRs can be found. As new ceramic systems, including more robust monolithic materials, are available in the market, it becomes imperative that further laboratory and clinical investigations including MCR as control are needed. To date, only 1 randomized controlled clinical trial involving 3- to 5-unit zirconia-supported fixed partial dentures has been performed with metal-ceramic as controls. The findings of this 3-year follow-up have shown no differences among biological or technical complications between the 2 systems. Chip-off fractures occurred in 25% of the zirconia-supported pros- theses and in 19.4% of the metal-ceramics. Although the chipping occurrence was not statistically different between the groups, only the zirconia-supported prostheses presented unacceptable major fractures of the veneering ceramic relative to the minor chips observed in the metal-ceramic system.69 NEW CONCEPTS FOR THE ALL-CERAMIC SYSTEMS Many manufacturers have shifted their attention to the development of monolithic all- ceramic materials to simply remove the most common failing layer of the system and to avoid inherent residual thermal stresses in bilayer all-ceramic systems. In combina- tion with CAD/CAM fabrication, monolithic/full-anatomic crown restorations seemed to be reliable and robust. Most recently, monolithic zirconia ceramic restorations refined with superficial glazing and staining and functionally graded glass/zirconia/ glass structures106 are being explored in high-load bearing areas. In addition, CAD/CAM capabilities creating separate core and veneer layers that could then be joined with nonthermal methods will continue to evolve and are of particular interest for extended restorations.107 Subtractive CAD/CAM approaches, removing material from a block to create a shape, will be complemented by additive approaches, depositing materials only in places where it is needed to form a restoration.74 Although issues are still remaining with each of these approaches, they show great promise. SUMMARY Fracture of the veneering ceramics, thermal interaction between core and ceramic materials, and susceptibility of zirconia to aging are still being debated in the dental liter- ature. Refinement of framework design and innovative CAD/CAM veneering techniques are promising tools to improve the clinical performance of zirconia-supported restora- tions. The use of monolithic leucite and lithium disilicate glass ceramic systems have shown promising laboratory and clinical results for small restorations such as inlays, onlays, crowns, and laminates. Further laboratory and clinical investigations using all- ceramic materials compared with metal-ceramic systems are strongly recommended. ACKNOWLEDGMENTS The authors thank the Department of Biomaterials and Biomimetics at the New York University College of Dentistry, USA. The authors also thank Dr Leonard Marotta (Marotta Dental Studios) for substantial collaboration. Special acknowledgment to Drs Van P. Thompson, Elizabeth Dianne Rekow and Joerg R. Strub for their support and professional guidance.
All-Ceramic Systems 347REFERENCES 1. Denry I, Holloway JA. Ceramics for dental applications: a review. Materials 2010;3:351–68. 2. Conrad HJ, Seong WJ, Pesun IJ. Current ceramic materials and systems with clinical recommendations: a systematic review. J Prosthet Dent 2007;98(5): 389–404. 3. Larsson C, Vult von Steyern P, Nilner K. A prospective study of implant- supported full-arch yttria-stabilized tetragonal zirconia polycrystal mandibular fixed dental prostheses: three-year results. Int J Prosthodont 2010;23(4):364–9. 4. Manicone PF, Rossi Iommetti P, Raffaelli L. An overview of zirconia ceramics: basic properties and clinical applications. J Dent 2007;35(11):819–26. 5. Della Bona A, Kelly JR. The clinical success of all-ceramic restorations. J Am Dent Assoc 2008;139(Suppl):8S–13S. 6. Al-Amleh B, Lyons K, Swain M. Clinical trials in zirconia: a systematic review. J Oral Rehabil 2010;37(8):641–52. 7. Land CH. Porcelain dental art. Dental Cosmos 1903;45:437–615. 8. McLean JW, Hughes TH. The reinforcement of dental porcelain with ceramic oxides. Br Dent J 1965;119:251–67. ¨ 9. Sjogren G, Lantto R, Granberg A, et al. Clinical examination of leucite-reinforced glass-ceramic crowns (Empress) in general practice: a retrospective study. Int J Prosthodont 1999;12(2):122–8.10. Denry I, Rosenstiel SF. Phase tranformation in feldspathic dental porcelains. In: Fischman G, editor. Bioceramics: materials and applications. Westervill (OH): The American Ceramic Society; 1995.11. Guazzato M, Albakry M, Ringer SP, et al. Strength, fracture toughness and microstructure of a selection of all-ceramic materials. Part I. Pressable and alumina glass-infiltrated ceramics. Dent Mater 2004;20(5):441–8.12. Dong JK, Luthy H, Wohlwend A, et al. Heat-pressed ceramics: technology and strength. Int J Prosthodont 1992;5(1):9–16.13. Kramer N, Taschner M, Lohbauer U, et al. Totally bonded ceramic inlays and onlays after eight years. J Adhes Dent 2008;10(4):307–14.14. Fradeani M, Redemagni M, Corrado M. Porcelain laminate veneers: 6- to 12- year clinical evaluation–a retrospective study. Int J Periodontics Restorative Dent 2005;25(1):9–17.15. Fradeani M, Redemagni M. An 11-year clinical evaluation of leucite-reinforced glass-ceramic crowns: a retrospective study. Quintessence Int 2002;33(7): 503–10. ¨16. Holand W, Schweiger M, Watzke R, et al. Ceramics as biomaterials for dental restoration. Expert Rev Med Devices 2008;5(6):729–45. ¨ 17. Holand W, Apel E, vant Hoen C, et al. Studies of crystal phase formation in the early stage crystallization of lithium disilicate glass-ceramics. J Non Cryst Solids 2006;352:4041–50. ¨18. Holand W, Schweiger M, Frank M, et al. A comparison of the microstructure and properties of the IPS Empress 2 and the IPS Empress glass-ceramics. J Biomed Mater Res 2000;53(4):297–303.19. Valenti M, Valenti A. Retrospective survival analysis of 261 lithium disilicate crowns in a private general practice. Quintessence Int 2009;40(7):573–9.20. Marquardt P, Strub JR. Survival rates of IPS empress 2 all-ceramic crowns and fixed partial dentures: results of a 5-year prospective clinical study. Quintes- sence Int 2006;37(4):253–9.
348 Guess et al 21. Guess PC, Strub JR, Steinhart N, et al. All-ceramic partial coverage restora- tions–midterm results of a 5-year prospective clinical splitmouth study. J Dent 2009;37(8):627–37. 22. Etman MK, Woolford MJ. Three-year clinical evaluation of two ceramic crown systems: a preliminary study. J Prosthet Dent 2010;103(2):80–90. 23. Wolfart S, Bohlsen F, Wegner SM, et al. A preliminary prospective evaluation of all-ceramic crown-retained and inlay-retained fixed partial dentures. Int J Pros- thodont 2005;18(6):497–505. 24. Wolfart S, Eschbach S, Scherrer S, et al. Clinical outcome of three-unit lithium- disilicate glass-ceramic fixed dental prostheses: up to 8 years results. Dent Mater 2009;25(9):e63–e71. 25. Fasbinder DJ, Dennison JB, Heys D, et al. A clinical evaluation of chairside lithium disilicate CAD/CAM crowns: a two-year report. J Am Dent Assoc 2010; 141(Suppl 2):10S–4S. 26. Haselton DR, Diaz-Arnold AM, Hillis SL. Clinical assessment of high-strength all- ceramic crowns. J Prosthet Dent 2000;83(4):396–401. 27. Sundh A, Sjogren G. A comparison of fracture strength of yttrium-oxide- partially-stabilized zirconia ceramic crowns with varying core thickness, shapes and veneer ceramics. J Oral Rehabil 2004;31(7):682–8. 28. Chai J, Takahashi Y, Sulaiman F, et al. Probability of fracture of all-ceramic crowns. Int J Prosthodont 2000;13(5):420–4. 29. Xiao-ping L, Jie-mo T, Yun-long Z, et al. Strength and fracture toughness of MgO-modified glass infiltrated alumina for CAD/CAM. Dent Mater 2002;18(3): 216–20. 30. Raigrodski AJ. Contemporary materials and technologies for all-ceramic fixed partial dentures: a review of the literature. J Prosthet Dent 2004;92(6):557–62. 31. Wassermann A, Kaiser M, Strub JR. Clinical long-term results of VITA In-Ceram Classic crowns and fixed partial dentures: a systematic literature review. Int J Prosthodont 2006;19(4):355–63. 32. Christel P, Meunier A, Dorlot JM, et al. Biomechanical compatibility and design of ceramic implants for orthopedic surgery. Ann N Y Acad Sci 1988;523:234–56. 33. Chevalier J. What future for zirconia as a biomaterial? Biomaterials 2006;27(4): 535–43. 34. Denry I, Kelly JR. State of the art of zirconia for dental applications. Dent Mater 2008;24(3):299–307. 35. Aboushelib MN, Dozic A, Liem JK. Influence of framework color and layering technique on the final color of zirconia veneered restorations. Quintessence Int 2010;41(5):e84–e89. 36. Degidi M, Artese L, Scarano A, et al. Inflammatory infiltrate, microvessel density, nitric oxide synthase expression, vascular endothelial growth factor expression, and proliferative activity in peri-implant soft tissues around titanium and zirco- nium oxide healing caps. J Periodontol 2006;77(1):73–80. 37. Rimondini L, Cerroni L, Carrassi A, et al. Bacterial colonization of zirconia ceramic surfaces: an in vitro and in vivo study. Int J Oral Maxillofac Implants 2002;17(6):793–8. 38. Garvie RC, Hannink RH, Pascoe RT. Ceramic steel? Nature 1975;258:703–4. 39. Christel P, Meunier A, Heller M, et al. Mechanical properties and short-term in- vivo evaluation of yttrium-oxide-partially-stabilized zirconia. J Biomed Mater Res 1989;23(1):45–61. 40. Piconi C, Maccauro G. Zirconia as a ceramic biomaterial. Biomaterials 1999; 20(1):1–25.
All-Ceramic Systems 34941. Meyenberg KH, Luthy H, Scharer P. Zirconia posts: a new all-ceramic concept for nonvital abutment teeth. J Esthet Dent 1995;7(2):73–80. ´42. Sturzenegger B, Feher A, Luthy H, et al. Clinical evaluation of zirconium oxide bridges in the posterior segments fabricated with the DCM system. Acta Med Dent Helv 2000;5:131–9.43. Komine F, Tomic M. A single-retainer zirconium dioxide ceramic resin-bonded fixed partial denture for single tooth replacement: a clinical report. J Oral Sci 2005;47(3):139–42.44. Bergler M, Holst S, Blatz MB, et al. CAD/CAM and telescopic technology: design options for implant-supported overdentures. Eur J Esthet Dent 2008; 3(1):66–88.45. Glauser R, Sailer I, Wohlwend A, et al. Experimental zirconia abutments for implant-supported single-tooth restorations in esthetically demanding regions: 4-year results of a prospective clinical study. Int J Prosthodont 2004;17(3): 285–90.46. Sailer I, Philipp A, Zembic A, et al. A systematic review of the performance of ceramic and metal implant abutments supporting fixed implant reconstructions. Clin Oral Implants Res 2009;20(Suppl 4):4–31.47. Andreiotelli M, Wenz HJ, Kohal RJ. Are ceramic implants a viable alternative to titanium implants? A systematic literature review. Clin Oral Implants Res 2009; 20(Suppl 4):32–47.48. Wenz HJ, Bartsch J, Wolfart S, et al. Osseointegration and clinical success of zirconia dental implants: a systematic review. Int J Prosthodont 2008;21(1):27–36.49. Larsson C, Vult von Steyern P, Sunzel B, et al. All-ceramic two- to five-unit implant-supported reconstructions. A randomized, prospective clinical trial. Swed Dent J 2006;30(2):45–53.50. Miyazaki T, Hotta Y, Kunii J, et al. A review of dental CAD/CAM: current status and future perspectives from 20 years of experience. Dent Mater J 2009; 28(1):44–56.51. Rekow ED. Dental CAD/CAM systems: a 20-year success story. J Am Dent Assoc 2006;137(Suppl):5S–6S.52. Tinschert J, Natt G, Hassenpflug S, et al. Status of current CAD/CAM technology in dental medicine. Int J Comput Dent 2004;7(1):25–45.53. Donovan TE. Factors essential for successful all-ceramic restorations. J Am Dent Assoc 2008;139(Suppl):14S–8S.54. Deville S, Chevalier J, Gremillard L. Influence of surface finish and residual stresses on the ageing sensitivity of biomedical grade zirconia. Biomaterials 2006;27(10):2186–92.55. Tholey MJ, Berthold C, Swain MV, et al. XRD(2) micro-diffraction analysis of the interface between Y-TZP and veneering porcelain: role of application methods. Dent Mater 2010;26(6):545–52.56. Kobayashi K, Kuwajima H, Masaki T. Phase change and mechanical properties of ZrO2-Y2O3 solid electrolyte after aging. Solid State Ionics 1981;3:489–93.57. Kelly JR, Denry I. Stabilized zirconia as a structural ceramic: an overview. Dent Mater 2008;24(3):289–98.58. Lawson S. Environmental degradation of zirconia ceramics. J Eur Ceram Soc 1995;15:485–502.59. Hannink R, Kelly PM, Muddle B. Transformation toughening in zirconia contain- ing ceramics. J Am Ceram Soc 2000;83(3):461–87.60. Kim JW, Covel NS, Guess PC, et al. Concerns of hydrothermal degradation in CAD/CAM zirconia. J Dent Res 2010;89(1):91–5.
350 Guess et al 61. Cehreli MC, Kokat AM, Akca K. CAD/CAM Zirconia vs. slip-cast glass-infiltrated Alumina/Zirconia all-ceramic crowns: 2-year results of a randomized controlled clinical trial. J Appl Oral Sci 2009;17(1):49–55. 62. Sailer I, Feher A, Filser F, et al. Five-year clinical results of zirconia frameworks for posterior fixed partial dentures. Int J Prosthodont 2007;20(4):383–8. 63. Beuer F, Edelhoff D, Gernet W, et al. Three-year clinical prospective evaluation of zirconia-based posterior fixed dental prostheses (FDPs). Clin Oral Investig 2009;13(4):445–51. 64. Roediger M, Gersdorff N, Huels A, et al. Prospective evaluation of zirconia posterior fixed partial dentures: four-year clinical results. Int J Prosthodont 2010;23(2):141–8. 65. Aboushelib MN, Feilzer AJ, Kleverlaan CJ. Bridging the gap between clinical failure and laboratory fracture strength tests using a fractographic approach. Dent Mater 2009;25(3):383–91. 66. Taskonak B, Yan J, Mecholsky JJ Jr, et al. Fractographic analyses of zirconia- based fixed partial dentures. Dent Mater 2008;24(8):1077–82. 67. Schmitter M, Mussotter K, Rammelsberg P, et al. Clinical performance of extended zirconia frameworks for fixed dental prostheses: two-year results. J Oral Rehabil 2009;36(8):610–5. 68. Ortorp A, Kihl ML, Carlsson GE. A 3-year retrospective and clinical follow-up study of zirconia single crowns performed in a private practice. J Dent 2009; 37(9):731–6. 69. Sailer I, Gottnerb J, Kanelb S, et al. Randomized controlled clinical trial of zirconia- ceramic and metal-ceramic posterior fixed dental prostheses: a 3-year Follow-up. Int J Prosthodont 2009;22(6):553–60. 70. Hobkirk JA, Wiskott HW. Ceramics in implant dentistry (Working Group 1). Clin Oral Implants Res 2009;20(Suppl 4):55–7. 71. Tsalouchou E, Cattell MJ, Knowles JC, et al. Fatigue and fracture properties of yttria partially stabilized zirconia crown systems. Dent Mater 2007;24(3):308–18. 72. Guess PC, Zhang Y, Thompson VP. Effect of veneering techniques on damage and reliability of Y-TZP trilayers. Eur J Esthet Dent 2009;4(3):262–76. 73. Bonfante EA, Rafferty B, Zavanelli RA, et al. Thermal/mechanical simulation and laboratory fatigue testing of an alternative yttria tetragonal zirconia polycrystal core-veneer all-ceramic layered crown design. Eur J Oral Sci 2010;118(2): 202–9. 74. Silva NR, Bonfante EA, Zavanelli RA, et al. Reliability of metalloceramic and zirconia-based ceramic crowns. J Dent Res 2010;89(10):1051–6. 75. Wolfart S, Harder S, Eschbach S, et al. Four-year clinical results of fixed dental prostheses with zirconia substructures (Cercon): end abutments vs. cantilever design. Eur J Oral Sci 2009;117(6):741–9. 76. Birkby I, Stevens R. Applications of zirconia ceramics. Key Eng Mater 1996; 122–124:527–52. 77. Swain MV. Unstable cracking (chipping) of veneering porcelain on all-ceramic dental crowns and fixed partial dentures. Acta Biomater 2009;5(5):1668–77. 78. Rues S, Kroger E, Muller D, et al. Effect of firing protocols on cohesive failure of all-ceramic crowns. J Dent 2010;38:987–94. 79. Pogoncheff CM, Duff RE. Use of zirconia collar to prevent interproximal porce- lain fracture: a clinical report. J Prosthet Dent 2010;104(2):77–9. 80. Marchack B, Futatsuki Y, Marchack C, et al. Customization of milled zirconia copings for all-ceramic crowns: a clinical report. J Prosthet Dent 2008;99(3): 163–73.
All-Ceramic Systems 351 81. Lorenzoni FC, Martins LM, Silva NR, et al. Fatigue life and failure modes of crowns systems with a modified framework design. J Dent 2010;38(8):626–34. 82. Rosentritt M, Steiger D, Behr M, et al. Influence of substructure design and spacer settings on the in vitro performance of molar zirconia crowns. J Dent 2009;37(12):978–83. 83. Tinschert J, Schulze KA, Natt G, et al. Clinical behavior of zirconia-based fixed partial dentures made of DC-Zirkon: 3-year results. Int J Prosthodont 2008; 21(3):217–22. 84. Nothdurft FP, Pospiech PR. Zirconium dioxide implant abutments for posterior single-tooth replacement: first results. J Periodontol 2009;80(12):2065–72. 85. Luthardt RG, Holzhuter MS, Rudolph H, et al. CAD/CAM-machining effects on Y-TZP zirconia. Dent Mater 2004;20(7):655–62. 86. Zhang Y, Lawn BR, Rekow ED, et al. Effect of sandblasting on the long-term performance of dental ceramics. J Biomed Mater Res B Appl Biomater 2004; 71(2):381–6. 87. Zhang Y, Lawn BR, Malament KA, et al. Damage accumulation and fatigue life of particle-abraded ceramics. Int J Prosthodont 2006;19(5):442–8. 88. Wang H, Aboushelib MN, Feilzer AJ. Strength influencing variables on CAD/ CAM zirconia frameworks. Dent Mater 2008;24(5):633–8. 89. Sato H, Yamada K, Pezzotti G, et al. Mechanical properties of dental zirconia ceramics changed with sandblasting and heat treatment. Dent Mater J 2008; 27(3):408–14. 90. Guazzato M, Quach L, Albakry M, et al. Influence of surface and heat treatments on the flexural strength of Y-TZP dental ceramic. J Dent 2005;33(1):9–18. 91. Kosmac T, Oblak C, Jevnikar P, et al. The effect of surface grinding and sand- blasting on flexural strength and reliability of Y-TZP zirconia ceramic. Dent Mater 1999;15(6):426–33. 92. Kosmac T, Oblak C, Jevnikar P, et al. Strength and reliability of surface treated Y-TZP dental ceramics. J Biomed Mater Res 2000;53(4):304–13. 93. Guess PC, Zhang Y, Kim JW, et al. Damage and reliability of Y-TZP after cemen- tation surface treatment. J Dent Res 2010;89(6):592–6. 94. Hickel R, Roulet JF, Bayne S, et al. Recommendations for conducting controlled clinical studies of dental restorative materials. J Adhes Dent 2007;9(Suppl 1): 121–47. 95. Kelly JR. Perspectives on strength. Dent Mater 1995;11(2):103–10. 96. Kelly JR. Clinically relevant approach to failure testing of all-ceramic restora- tions. J Prosthet Dent 1999;81(6):652–61. 97. Suttor D, Bunke K, Hoescheler S, et al. LAVA–the system for all-ceramic ZrO2 crown and bridge frameworks. Int J Comput Dent 2001;4(3):195–206. 98. Coelho PG, Bonfante EA, Silva NR, et al. Laboratory simulation of Y-TZP all-ceramic crown clinical failures. J Dent Res 2009;88(4):382–6. 99. Guess PC, Zavanelli RA, Silva NR, et al. Monolithic CD/CAM lithium disilicate versus veneered Y-TZP crowns: comparison of failure modes and reliability after fatigue. Int J Prosthodont 2010;23:434–42.100. Coelho PG, Silva NR, Bonfante EA, et al. Fatigue testing of two porcelain- zirconia all-ceramic crown systems. Dent Mater 2009;25(9):1122–7.101. Drummond J, Eliades G. Ceramic behavior under different environmental and loading conditions. Dental materials in vivo: aging and related phenomena. Chicago: Quintessence; 2003.102. Wolf D, Bindl A, Schmidlin PR, et al. Strength of CAD/CAM-generated esthetic ceramic molar implant crowns. Int J Oral Maxillofac Implants 2008;23(4):609–17.
352 Guess et al 103. Pjetursson BE, Sailer I, Zwahlen M, et al. A systematic review of the survival and complication rates of all-ceramic and metal-ceramic reconstructions after an observation period of at least 3 years. Part I. Single crowns. Clin Oral Implants Res 2007;18(Suppl 3):73–85. 104. Sailer I, Pjetursson BE, Zwahlen M, et al. A systematic review of the survival and complication rates of all-ceramic and metal-ceramic reconstructions after an observation period of at least 3 years. Part II. Fixed dental prostheses. Clin Oral Implants Res 2007;18(Suppl 3):86–96. 105. Napankangas R, Raustia A. Twenty-year follow-up of metal-ceramic single crowns: a retrospective study. Int J Prosthodont 2008;21(4):307–11. 106. Zhang Y, Kim JW. Graded structures for damage resistant and aesthetic all-ceramic restorations. Dent Mater 2009;25(6):781–90. 107. Beuer F, Schweiger J, Eichberger M, et al. High-strength CAD/CAM-fabricated veneering material sintered to zirconia copings–a new fabrication mode for all-ceramic restorations. Dent Mater 2009;25(1):121–8. 108. Groten M, Huttig F. The performance of zirconium dioxide crowns: a clinical follow-up. Int J Prosthodont 2010;23(5):429–31. 109. Schmitt J, Wichmann M, Holst S, et al. Restoring severely compromised anterior teeth with zirconia crowns and feather-edged margin preparations: a 3-year follow-up of a prospective clinical trial. Int J Prosthodont 2010;23(2):107–9. 110. Tsumita M, Kokubo Y, Ohkubo C, et al. Clinical evaluation of posterior all- ceramic FPDs (Cercon): a prospective clinical pilot study. J Prosthodont Res 2010;54(2):102–5. 111. Crisp RJ, Cowan AJ, Lamb J, et al. A clinical evaluation of all-ceramic bridges placed in UK general dental practices: first-year results. Br Dent J 2008;205(9): 477–82. 112. Raigrodski AJ, Chiche GJ, Potiket N, et al. The efficacy of posterior three-unit zirconium-oxide-based ceramic fixed partial dental prostheses: a prospective clinical pilot study. J Prosthet Dent 2006;96(4):237–44. 113. Schmitt J, Holst S, Wichmann M, et al. Zirconia posterior fixed partial dentures: a prospective clinical 3-year follow-up. Int J Prosthodont 2009;22(6):597–603. 114. Vult von Steyern P, Carlson P, Nilner K. All-ceramic fixed partial dentures designed according to the DC-Zirkon technique. A 2-year clinical study. J Oral Rehabil 2005;32(3):180–7. 115. Edelhoff D, Florian B, Florian W, et al. HIP zirconia fixed partial dentures–clinical results after 3 years of clinical service. Quintessence Int 2008;39(6):459–71. 116. Molin MK, Karlsson SL. Five-year clinical prospective evaluation of zirconia- based Denzir 3-unit FPDs. Int J Prosthodont 2008;21(3):223–7.